DOTTORATO DI RICERCA IN
Magnetic Nanoparticles as a multivalent
scaffold for biomedical applications
1. Introduction 1
2. Synthesis of MNPs 16
2.1 Synthesis with FeOOH 17
2.2 Synthesis with iron(III) oleate 22
2.3 Synthesis of magnetite MNPs with Iron Acetylacetonate 31 2.3.1 Synthesis of MNPs exploiting the seed mediated growth 32
2.3.2 Synthesis of larger magnetite MNPs from iron(III) 38 acetylacetonate
3. The α-Tn antigen mimetic and functionalization of MNPs 49
3.1 The α-Tn antigen 49
3.2 Synthesis of the α-Tn antigen mimetic 2 51
3.3 Synthesis of the linker 5 57
3.4 Synthesis of the α-Tn like derivative 3 : coupling reaction and 58 phosphonate insertion.
3.5 Functionalization of MNPs with the α-Tn antigen mimetic 3 59 4. Synthesis of negative control for biological tests for macrophage 65 activation
4.1 Synthesis of the glucose derivative for MNPs functionalization 66 4.2 Functionalization of MNPs with citrate, glucose and PEG 70
5. Macrophages activation 77
5.1 Macrophages role in the immune response 77
6. Functionalization of MNPs 90
6.1 Aminosilane functionalization 92
6.2 Synthesis of aminophosphonic linker 39 97
7. Conclusion and perspectives 102
8. Experimental section 105
8.1 Synthesis of MNPs 106
8.2 Functionalization of MNPS 109
8.3 Synthesis of linker 5 112
8.4 Synthesis of α-Tn antigen mimetic 3 113
8.5 Synthesis of glucose derivative 24 122
8.6 Synthesis of amino-phosphonate linker 39 126 8.7 Biological tests on macrophages activation 130
8.8 Structural characterization of MNPs 134
8.9 Magnetic and hyperthermic characterization 135
1 1. Introduction
The reduction of materials to the nanometric size, in the last decades has been the focus of intense research. Indeed, nanomaterials possess attractive properties which can be used, and in some cases are already in use, in many field of applications: catalysis, data storage, sensors and biomedicine . In particular, the application of nanomaterials in biology and medicine is receiving considerable attention, as they hold great promises on improving health care and advancing medical research .
Among the others, magnetic nanoparticles (MNPs) with size below 100 nm represent one of the most promising class of materials, thanks to their peculiar properties. The first prominent feature which makes magnetic nano-objects appealing for biomedical applications is represented by their controllable sizes ranging from few nanometres up to tens of nanometres, which are smaller or comparable to those of many biological entities, ranging from a single gene (2 nm wide and 10-100 nm long) to an entire cell (10-100 µm). The possibility of a interaction between such entities at the nanometric scale has progressively attracted the attention of many research groups all over the world [2a-b]. Beside their size, the importance of MNPs in the field of biomedicine relies on their specific properties, the most significant being superparamagnetism . When ferro- or ferrimagnetic particles belong to the nanometric size range they become single domain, i.e. the formation of magnetic domains is no longer energetically favoured, therefore they are characterized by a single magnetic moment given by the sum of all the atomic spins comprised in the nanoparticle . This magnetic moment will freely fluctuate like in a paramagnet (superparamagnetism) or will be blocked along certain favoured crystallographic directions (ferromagnetic-like behaviour) depending on whether the thermal energy is larger or smaller than the energy barrier separating that directions. This energy barrier is determined by the magnetic anisotropy of the material itself and, as a first approximation, is proportional to the volume of the MNPs .
These outstanding properties confer to MNPs unique sensing, moving and heating characteristic which can be exploited for bio-analysis or for the early diagnosis and therapy of several diseases.
It is worthy of noting that for biomedical application, biocompatibility is another mandatory requirement, restricting the choice for the inorganic core of the MNPs to iron oxides and in particular magnetite or maghemite .
At present, most applications of MNPs are based on the following physical principles [1a, 2b]:
the application of controlled magnetic field gradients for remotely direct MNPs towards organs or tissues or for moving MNPs tagged biomaterials; the utilization of the magnetic moment of the MNPs to modify the nearby
proton nuclear resonance (contrast agent (CA) for Magnetic Resonance Imaging (MRI));
the excitation of MNPs with an external alternating magnetic field inducing an heat release which can be used to selectively destroy tumour cells, exploiting their higher sensitivity to a temperature increase than healthy tissues (magnetic fluid hyperthermia, MFH).
For example, MNPs can help in the separation of selected biological entities from their native environment, so that concentrated samples may be prepared for subsequent analyses or other uses. This process involves two steps: 1) the tagging or labelling of the desired biological entity with the magnetic material and 2) the separation of these tagged entities via a fluid-based magnetic separation device. The tagging is possible by coating MNPs with suitable functional groups which in turn can provide a selective linkage to the target site exposed by a cell or a molecule, and at the same time maintain an optimal colloidal stability. A specific binding to the target can be achieved by using antibodies or other biological macromolecules such as hormones or folic acid [6,2b]. The magnetically labelled material can be then separated from its native solution by passing the fluid mixture through a region in which a magnetic field gradient is present, so that the tagged material is immobilized while the unwanted material is removed, as displayed in Figure 1.1.
Figure 1.1 : Standard methods for magnetic separation: a) the magnet is attached to the container wall of a solution of magnetically tagged (●) and unwanted (○) biomaterials. b) a solution containing tagged and unwanted biomaterials flows continuously through a region of strong magnetic field gradient, which captures the tagged particles.
In the field of sensing, MRI, is the area in which MNPs have found their major application, since they are capable of enhancing the contrast of the image (contrast agents). MRI provides images of the density distribution of protons or other nuclei through the application of appropriate magnetic field gradients and radiofrequency pulse sequences. MRI exploits the contrast created by different nuclear spin-spin (T2) and spin-lattice (T1) relaxation times found in different parts of the material to obtain images that can evidence specific differences . This technique is widely used in medical clinic to investigate the anatomy and physiology of the body. From the obtained images it is possible to evidence local pathologies and disease like tumour lesions, edemas, soft tissue damages, muscle lesions and many more.
Contrast agents are used in order to increase the natural contrast between healthy and pathological tissues and they normally act decreasing the relaxation times, T1 and T2, of the neighbour protons. At present, the most used CAs are based on paramagnetic gadolinium complexes,  which increase the contrast by
fluid flow fluid flow a) b) magnetic field remove magnetic field
decreasing T1 . However, CAs based on dextran coated assembly of superparamagnetic maghemite nanoparticles with a total average diameter between 20 and 150 nm are also commercially available. In Table 1.1 some examples of clinically approved CA for MRI are reported .
Generic Name Metal Trade Name
Ferumoxides Fe3O4 Endorem®, Fedirez®
Ferumoxyl Fe3O4 Lumirem®, GastroMARK
Ferucarbotran Fe3O4 Resovist®
Ferumoxtran Fe3O4 Sinerem®, Combidex®
Table 1.1 : Clinically approved CA for MRI based on magnetite nanoparticles [9a].
Ferrite MNP based CAs perform their function affecting the T2 relaxation time of the protons in the nearby tissues, leading to a better contrast in the acquired images. The advantages offered by MNPs-based CA, in comparison with conventional gadolinium chelates, rely on the enhanced cellular internalization and slower clearance from tumour site . In particular, for MNPs with diameters greater than 50 nm the cellular internalization is essentially due to the uptake by the cells of the reticuloendothelial system (RES), whereas nanoparticles with a diameter lower than 50 nm benefit from slower opsonization and RES clearance . In all of these cases the tissue distribution of the MNPs relies on a passive targeting rather than a direct labelling. Indeed, one of the most challenging opportunities is to functionalize the nanoparticles with specific biomolecules (monoclonal antibodies, peptides, or other target bioactive molecules) in order to direct the CA only to the desired target exploiting a receptor-mediated endocytosis and hence increasing a local accumulation in the diseased tissues . This would allows both the increase of the sensitivity of the technique and the reduction of the amount of contrast agent required to acquire an MRI image.
Finally, MNPs can be used as heat mediators in the hyperthermic treatment of tumour cells, which is a technique that is progressively acquiring more and more
relevance in the fight against tumour pathologies [2a,2b]. Hyperthermia is a general term which groups together several techniques, all based on the rise of temperature above the physiologic level (in the range of 40-45°C) within a targeted tumour without damaging the surrounding healthy tissues [9a]. The most extended method for increasing temperature above the systemic values is based on the application of microwaves , although therapies involving ionizing radiation  have also been successfully applied to destroy malignant tissues. The disadvantages of these strategies are related to undesired collateral effects such as ionization of genetic material (radiation) or lack of selectiveness (microwaves) that affect the surrounding healthy tissues . Another emerging hyperthermic treatment of tumours relies on the application of a radiofrequency on magnetic needles directly implanted into the target site [16.]; although very promising, this technique is invasive and its effectiveness is rather limited.
In this respect inorganic nanoparticles, which, in principle can be localized only at the tumour site, can represent a viable alternative. For example, successful
in vitro and in vivo studies have been reported on the use of functionalized gold
nanorods to convert infrared radiation (IR) into heat that selectively destroys cancer cells . The use of these kind of nanostructures for hyperthermia could be useful to avoid damages on healthy cells. On the other hand, IR radiation has a low penetration depth into human tissues, which limits this technique to surface applications, like melanoma cells [9a]. The employment of MNPs as heat mediators for MFH can help to overcome these drawbacks. In this case the temperature increasing is realized by means of an external alternating magnetic field acting on MNPs at the targeted site, which provides to the particle’s magnetic moment the energy required to overcome the barrier generated by the magnetic anisotropy. This energy is then released as heat which is dissipated to the surrounding tissues. MNPs can be accumulated in tumour tissues thanks to the so called enhance permeability and retention (EPR) effect . This mechanism relies on leaky vasculature characterizing cancerous tissues, which allows macromolecules and nanoparticles to extravasate and accumulate more readily. This passive targeting can be exploited to induce a local temperature enhancement and, as a consequence to selectively induce tumour cells death. The feasibility of MFH has been already demonstrated in clinical trials by the group of Prof. Jordan at Berlin’s Charité Hospital, who reported significant benefits in the treatment of recurrent glioblastoma multiforme and, more recently of prostate and pancreas tumours by using a combination of radiotherapy and heating produced by 12 nm
amino-silane coated Fe3O4 MNP directly implanted in the tumour mass at high
doses (ca. 50 mg/cm3) . As it can be inferred from the above description, an improvement of the hyperthermic treatment can be accomplished by the use of tumour targeted MNPs in order to increase the selectivity and reach the temperature enhancement with as low as possible amount of MNPs. Furthermore hyperthermia can be used in combination with other cancer therapies like chemotherapy and radiotherapy so as to increase their efficacy during the treatment. Moreover, chemotherapeutic drugs can be eventually linked to the MNPs used for the hyperthermic treatment and released only at the target site [9a, 1a].
We have described the appealing properties offered by MNPs that can be exploited in the field of biomedicine and, in particular, in the treatment and diagnosis of tumour pathologies. However, the most attracting feature is that all the above cited functionalities, i.e. sensing, moving and heating, can be combined in a unique multifunctional nano-object which ideally can ensure early diagnosis, deliver of the treatment to the specific target site at the right dose and time, and monitoring of the therapeutic effect. This kind of system will thus work as a diagnostic tool and as therapeutic agent, paving the way towards the so-called theranostic approach (therapeutic + diagnostic). In Figure 1.2 is provided a schematic representation of multifunctional MNPs, consisting essentially of:
1) a nanometric inorganic magnetic core; 2) an organic biocompatible coating;
3) a biologically active entity (a protein, an antibody, a small molecule)
Figure 1.2 : Theranostic multifunctional MNPs can act simultaneously as diagnostic tools and as therapeutic agents.
Considering this particular aspect we can appreciate the importance that a specific functionalization of MNPs could have in the development of an efficient tool for theranostic applications. For this purpose it is fundamental to develop a specific coating capable to make MNPs biocompatible and highly stable in physiological conditions so as to prolong their circulation time and the possibility to reach the target-cells [1a].
Another fundamental feature offered by MNPs is that they can represent a suitable scaffold for the multivalent exposition of biomolecules, which is essential for their interaction with biological entities, as indeed required in biomedicine. Multivalent interactions are characterized by the simultaneous binding of multiple ligands on a biological entity (a molecule or a surface), to multiple receptors on another. These interactions are very common in biology and have a number of characteristics that monovalent interactions do not possess . Multivalent interactions are usually based on not covalent bonds, such as hydrogen bonds, metal-ligand coordination, hydrophobic interactions and ionic bonds, which are all characterized by low energy and low specificity. However, increasing the number of the interactions, they become efficient and specific. Multivalent interactions can be collectively much stronger than the corresponding monovalent interactions thus providing many advantages.
Therapy Diagnosis Antibody Bioactive molecule Magnetic core Organic coating
Figure 1.3 : Ligand - Receptors interactions : monovalent interactions compared to multivalent interactions.
In a multivalent system the intensity of the signal can be simply varied by changing the number of ligand-receptors couples involved in the interaction. The signal modulation has a crucial role in biology, because the communications between biological entities do not rely on a on-off mechanism, and the biological answer to any environment alteration must be finely tuned. Moreover, multivalent interactions can induce morphological macroscopic modifications in cells during communication, thus improving the efficiency of the process.
A perfect example of this signal modulation is represented by the role that macrophages play in the immune response towards pathogenic organism. Indeed, macrophages, are able to engulf and then digest a bacterium only after the interaction with two or more antibodies takes place, (Figure 1.4) avoiding an immune response in the case of a single antibody bonding.
Figure 1.4 : Macrophages engulf pathogen organism after an antibodies multivalent interaction. The opsonization process marks the bacterium with specific opsonins enhancing phagocytosis. After the internalization, the bacteria will be digested in lysosomes (see Chapter 5).
Besides the adhesion of a bacteria to the surface of a cell, multivalent interactions are involved in many other biological processes, as for example, the adhesion of viruses to host cells, the interaction with toxins or antibodies, or the cell-cell communication (Figure 1.5). Some notable practical examples are provided by the interaction of influenza virus with bronchial epithelia cells  or the lectine-carbohydrate recognition which is the basis of most of the cell-cell recognition processes . Extracellular bacteria Macrophage Opsonization Internalization by macrophage digestion in lysosome Cell adhesion Cell Virus Antibodies Bacteria Toxins
Figure 1.5 : Examples of multivalent interactions in biological systems between a cell and toxins, bacteria, antibodies, viruses or other cells.
From the scenario described above it clearly emerges that MNPs decorated in a multivalent manner with biologically active molecules may hold great importance in selective targeting and in the development of novel theranostic tools for specific pathologies. In fact the magnetic core of MNPs represents a very promising multivalent scaffold. Indeed, if on one hand the multivalent presentation of specific epitopes to the immune cells can pave the way towards the application in immunotherapy and in particular in the development of antigen-specific vaccines , on the other the combination with the unique sensing, moving and heating properties provided by MNPs, can significantly enlarge the number of diagnostic and therapeutic functionalities conjugated in the same nanosystem.
As a matter of fact, immunotherapy has emerged as a powerful strategy in the fight against tumours and, the development of therapeutic vaccines using synthetic antigens, as immunogens, is becoming the ultimate goal in this field. Indeed, tumours uniquely or excessively express antigens (Tumour-Associated Antigens, TAAs) and, in particular, glycan antigens (Tumour-Associated Carbohydrate Antigens, TACAs), which can be useful targets for vaccines. TACAs are indeed widely exposed on cancer cell surfaces and their expression often correlates with cancer developmental stages, including invasion and metastasis. Furthermore, an abnormal glycosylation in the primary tumours is considered a signal of poor prognosis . Despite the large numbers of TAAs/TACAs so far described, their use in tumour therapy remains limited and needs some improvements. This is not only because immune responses in cancer patients can be relatively weak, but also because TACAs are poorly immunogenic antigens. Moreover, most TACAs are recognized as self and, according to their saccharidic nature, they cannot be presented to T cells for T cell responses (T cell independent type II antigens). Consequently, the class switch from IgM to IgG and the recall memory response are not generated . IgM (immunoglobulin M) is a type of antibody produced by B cells, and it is the first antibody elicited in response to initial exposure to an antigen; IgG (immunoglobulin G) are also produced by B cells but represent the long term response of the body to a disease. IgM are short term, disappear after a few weeks and they are then replaced by IgG that provide a long lasting immunity . A successful strategy to overcome the limitations mentioned above, might be mimicking the natural multivalent approach of the molecular biosystems by binding carbohydrate antigens to multivalent scaffolds, such as nanomaterials. TACA multivalent display, indeed, mimicking the natural multivalent carbohydrate presentation on a cell surface, can lead to B cell
activation and antibody production . Furthermore, a nanomaterial, as antigen delivery system, can provide an adjuvant activity, inducing the activation and maturation of antigen presenting cells (APCs),  thus promoting the antigen cross-presentation . All these events are essential for the induction of an efficient antitumour immune response.
In this context, the main target of this thesis has been the synthesis and characterization of a novel glycoconjugate nanosystem composed by magnetite MNPs functionalized with a synthetic, conformationally rigid mimetic of the α-Tn antigen , that is a TACA expressed in carcinoma-associated mucins , for application in immunotherapy. The evaluation of the immunoactivity of the glycosylated MNPs was accomplished by means of in vitro tests on the activation of macrophages. The choice of macrophages is based on the fact that they represent a perfect “bridge” between the innate immunity and the adaptive immunity and play a crucial role in the activation and amplification of the immune response .
In addition, since this work was aimed at the development of a multifunctional magnetic nanosystem, important efforts were devoted to the development of a suitable synthetic procedure for obtaining MNPs with optimized physical and chemical properties for their application in nanomedicine.
For the synthesis of MNPs we exploited the thermal decomposition of metal-organic precursors in high boiling solvent . Several attempts were performed in order to obtain highly crystalline, pure magnetite MNPs with a size in the 12-15 nm range varying the experimental parameters like the nature of the metal-organic precursor, the amount and kind of surfactants, the solvent, or the heating ramp. This particular size corresponds to the best compromise between a large heating efficiency in magnetic fluid hyperthermia and colloidal stability.
Finally, in order to make the proposed approach more versatile, we explored diverse functionalization methods, by changing the bifunctional linker used to link the saccharidic epitope onto the surface of the MNPs. We thus obtained nanosystems with suitable water solubility and suitable to be further coupled with bioactive molecules. In particular, we synthesized a new bifunctional linker derived from hexaethylene glycol to confer to MNPs the desired solubility and reactivity towards further functionalization.
For a better comprehension of this PhD work a brief summary is reported here after:
in Chapter 2, the experiments performed for MNPs synthesis, changing the precursor for the thermal decomposition and the reaction conditions, in order to optimize their structural and physical properties, are described; Chapter 3 is dedicated to the α-Tn antigen mimetic, from its synthesis to the
bonding to the magnetite MNPs;
in Chapter 4 it is described the preparation of functionalized MNPs samples used as negative controls for the biological tests on the macrophages activation, in order to better evaluate the effect of MNPs decorated with the α-Tn antigen mimetic on immune cells;
in Chapter 5 the above mentioned biological tests on macrophages activation are described in detail;
Chapter 6 is focused on the study of bifunctional ligands for MNPs functionalization in order to render them suitable for further decoration with bioactive molecules. We describe the functionalization of MNPs with an aminosilane ligand and then the synthesis of a new bifunctional ligand derived from hexaethylene glycol bearing two diverse functional groups: a phosphonate group at one end and an amino group at the other;
conclusions and future perspective are exposed in Chapter 7;
in Chapter 8 all the experimental data and the descriptions of the characterization techniques are reported.
 (a) A. G. Roca, R. Costo et al., J. Phys. D:Appl. Phys., 2009, 42, 224002; (b) P. Tartaj, M.P. Morales et al., J. Phys. D: Appl. Phys., 2003, 36 R182.
 (a) Q. A. Pankhurst, N. K.T. Thanh et al., J. Phys. D: Appl. Phys., 2009 42, 224001; (b) Q.A. Pankhurst, J. Connolly et al., J. Phys. D: Appl.Phys., 2003, 36, R167; (c) for magnetic biosensors: J.B. Haun,T.J. Yoon et al., Nanomed.
Nanobiotechnol., 2010, 2, 291; (d) C.T.Yavuz, J.T. Mayo et al., Science, 2006, 314, 964.
 (a) D. Jiles, Introduction to Magnetism and MagneticMaterials (London: Chapman and Hall), 1991; (b) A. H. Morrish, The Physical Principles of
Magnetism,(New York: IEEE Press), 2001; (c) J. M. D. Coey, Magnetism and Magnetic Materials, Cambridge Univ. Pr. (2010).
 E. C. Stoner, E. P. Wohlfarth; Philosophical Transaction of the Royal Society A, 1948, 240, 599.
 J. Sun et al, J. Biomed. Mater. Res. A, 2007, 80A, 333; (b) A. K. Gupta and S. Wells, IEEE Trans. Nanobiosci, 2004, 3, 66; (c) B. Ankamwar; T. C. Lai; J. H. Huang; R. S. Liu; M. Hsiao; C. H. Chen and Y. K. Hwu, Nanotechnology, 2010, 21 075102 (9pp).
 D. Högemann; L. Josephson; R. Weissleder and J. P. Basilion, Bioconjugate Chem. 2000, 11, 941; (b) L. Levy, Y. Sahoo; K. S. Kim; E. J. Bergey and P. N.
Prasad, Chem. Mater., 2002, 14, 3715; (c) Y. Zhang, N. Kohler and M. Zhang,
Biomaterials, 2002, 23, 1553.
 (a) P. C. Lauterbur, Nature, 1973, 242, 190; (b) P. Mansfield; P. G. Morris, NMR imaging in biomedicine, Suppl.2 Adv. Mag. Res., Academic Press, 1982; (c)
C. Guy; D. Ffytche, An introduction to the principles of medical imaging, Imperial College Press eds.London, 2000.
 (a) S. Laurent; L.Van der Elst et al., Helv.Chim.Acta, 2000, 83, 394; (b) S. Laurent; D. Forge et al., Chem. Rev., 2008, 108, 2064; (c) E. Taboada; R. Solanas
14  (a) G. F. Goya; V. Grazú; M. R. and Ibarra, Current Nanoscience, 2008, 4, 1 (b) D. Pouliquen, H. Perroud et al., Mag.Res.Med., 24, p. 75 (1992); b) W. Reith, M. Forsting et al., Am. J. Neuroradiol., 16, p. 53 (1995).
 (a) W. S. Enochs; F. Harsh; F. Hochberg and R. Weissledher, J. Magn. Reson. Imaging, 1999, 9, 228; (b) P. Varallyay; G. Nesbit; L. L. Muldoon; R. R. Nixon; J.
I. Delashaw; J. I. Cohen; A. Petrillo; D. Rink and E. A. Neuwelt, AJNR Am. J.
Neuroradiol., 2002, 23, 10.
 S. E. Barry, Int. J. Hyperthermia., 2008, 24, 451.
 C. Sun; J. S. H. Lee and M. Zhang, Adv. Drug Del. Rev., 2008, 60, 1252.  R. A. Gardner; H. I. Vargas; J. B. Block; C. L. Vogel; A. J. Fenn; G. V. Kuehl; M. Doval, Ann. Surg. Oncol., 2002, 9, 326.
 (a) H. H. Kampinga, Int. J. Hyperthermia, 2006, 22, 191; (b) C. F. Gottlieb; G. B. Seibert; N. L. Block, Radiology, 1988, 169, 243.
 (a) D. L. Cockroft,; D. A. T. New, Nature, 1975, 258, 604; (b) X. He; S. McGee; J. E. Coad; F. Schmidlin; P. A. Iaizzo; D. J. Swanlund; S. Kluge; E. Rudie; J. C. Bischof, Int. J. Hyperthermia, 2004, 20, 567.
 K. F. Chu and D. E. Dupuy, Nature Reviews Cancer, 2014, 14, 199.
 (a) L. F. de Freitas; L. C. Zanelatto; L. M. S. Mantovani; P. B. G. Silva; R. Ceccini; C. Grecco; L. T. Moriyama; C. Kurachi; V. C. A. Martins and A. M. G. Plepis, Laser Phys., 2013, 23, 066003; (b) X. Huang; I. H. El-Sayed; W. Qian; M. A. El-Sayed, J. Amer. Chem. Soc., 2006, 128, 2115.
 (a) H. Maeda; Advances in Enzyme Regulation, 2001, 41, 189; (b) O. Clement; N. Siauve; M. Lewin; E. de Kerviler; C.A. Cuenod; G. Frija, Biomedicine and
Pharmacotherapy, 1998, 52, 51.
 K. Maier-Hauff; F. Ulrich; D. Nestler; H. Niehoff; P. Wust; B. Thiesen; H. Orawa; V. Budach and A. Jordan, J. Neurooncol., 2011, 103, 2, 317.
 M. Mammen; S.-K. Choi; G. M. Whitesides, Angew. Chem., Int. Ed., 1998, 37, 2754.
15 a) W. J. Lees; A. Spaltenstein; W. J. E. Kingery; G. M. Whitesides, J. Med.
Chem., 1994, 37, 3419.
 H. Lis; N. Sharon, Chem. Rev., 1998, 98, 637.
 (a) B. L. Wilkinson; S. Day; L. R. Malins; V. Apostolopoulos; R. J. Payne, Angew. Chem. Int. Ed., 2011, 50, 1635; (b) S. Grigalevicius; S. Chierici; O.
Renaudet; R. Lo-Man; E. De´riaud; C. Leclerc; P. Dumy, Bioconjugate Chemistry, 2005, 16, 1149; (c) Q. Li; M. R. Anver; D. O. Butcher; J. C. Gildersleeve; Mol.Cancer Ther., 2009, 8, 971; (d) G. F. Springer; P. R. Desai; H. Tegtmeyer; B.
D. Spencer; E. F.Scanlon, Ann. N. Y. Acad. Sci. 1993, 690, 355; (d) G. F. Springer; P. R. Desai; W. Wise; S. C. Carlstedt; H.Tegtmeyer; H. Stein, E. F. Scanlon in
Immunodiagnosis of Cancer, 2nd ed. (Eds.: R. B. Herberman, D.W. Mercer),
MarcelDekker, New York, 1990, 587.
 Z. Guo and Q. Wang, Curr. Opin.Chem. Biol., 2009, 13, 608.  C. C. Liu and X. S. Ye, Glycoconjugate J., 2012, 29, 259.
 A. K. Abbas; A. H. Lichtman, Basic Immunology: : Functions and Disorders of the Immune System, Saunders; 3 edition (February 12, 2010).
 A. L. Parry; N. A. Clemson; J. Ellis; S. S. Bernhard; B. G. Davis and N. R. Cameron; J. Am. Chem. Soc., 2013, 135, 9362.
 S. T. Reddy; M. A. Swartz and J. A. Hubbell, Trends Immunol., 2006, 27, 573.  S. Hirosue; I. C. Kourtis; A. J. van der Vlies; J. A. Hubbell and M. A. Swartz; Vaccine, 2010, 28, 7897.
 T. Ju; V. I. Otto; R. D. Cummings, Angew. Chem. Int. Ed., 2011, 50, 1770.  M. A.Hollingsworth; B. J. Swanson, Nature Reviews Cancer, 2004, 4, 45.  S. Sun; H. Zeng; J. Am. Chem. Soc., 2002, 124 (28), 8204.
2. Synthesis of MNPs
Nowadays, there is a great interest in the use of MNPs in various field of application, from engineering to nanobiotecnology and biomedicine . The critical dependence of their physical properties on the particle size, shape and structure if on one hand allows for a fine tuning of their behaviour, on the other requires a tight control at the synthetic level. As a consequence, a wealth of methods of synthesis has been developed to answer to the different need arising from the different applications meanwhile granting a fine control on the morphological properties. In the literature many procedures are described concerning the bottom-up approach and most of them are focused on the thermal decomposition of a precursor (metal-organic or inorganic salts) in the presence of surfactants in high boiling solvents . It is worth to note that the thermal decomposition method is one of the best in terms of crystallinity, size distribution and magnetic properties of the final product, particularly if compared with the co-precipitation method, the sol-gel processes or the synthesis in reverse micelles. Thanks to these advantages thermal decomposition has rapidly gained a large popularity, becoming one of the most common method for the production of MNPs . However, despite of its large popularity, this technique is still suffering some drawbacks in terms of reproducibility, phase homogeneity and size or composition control. The main hurdle found by each "nanoparticle-chemist" is to reproduce in his own laboratory the procedure illustrated in a paper getting the same results. This is mainly due to the great number of experimental variables that must be simultaneously controlled in the reaction set-up, like the temperature increasing rate, the stirring rate, the nitrogen flow and many others. Each one of them affects the nature and the quality of the final product, thus it is essential to set all the parameters in order to obtain the desired product .
In this work the thermal decomposition process has been chosen as the principal way to obtain good quality magnetite MNPs exploitable for our purpose. In the following paragraph the attempts to synthesize iron oxide MNPs with a diameter of about 12-15 nm varying the nature of the precursor and the experimental conditions will be described. For each precursor many experiments were performed in order to analyze the dependence of the MNPs behaviours on the experimental parameters and thus find the best reaction conditions.
2.1 Synthesis with FeOOH
The first precursor tested for the thermal decomposition reaction was the iron (III) oxide hydrate, FeOOH in the presence of oleic acid as surfactant and
octadecene as high boiling solvent (b.p. 320°C). The MNPs were prepared following a procedure similar to that reported by Xue et al .
Precursor Surfactant Solvent
FeOOH Oleic Acid 1-Octadecene
Different samples were prepared by varying the reaction conditions (Table 2.1). However the increasing temperature rate and the length of the final step at 300°C were always kept constant in all syntheses and equal to 10°C/min up to 180°C and 6°C/min up to 300°C (Figure 2.1). All samples were recovered from the reaction mixture by magnetic decantation followed by several washing/precipitating steps. Details of the preparation are given in the experimental section.
The reaction was first carried out at a 1:4 precursor/surfactant concentration ratio under inert atmosphere. The as prepared MNPs IOMNP1 have an XRD pattern compatible with a mixed phase composed by a 53% of the cubic inverse spinel structure of magnetite (PDF 89-0691) maghemite (PDF 39-1346) or any partially oxidized intermediate ferrite phase, which cannot be discriminated from each other by this technique and by a 47% of the rhombohedral structure of
surfactant Precursor conc. (mg/mL)
IOMNP1 1/4 28.5 Inert (N2)
IOMNP2 1/5.5 7.2 Inert (N2)
IOMNP3 1/5.5 7.2 Air
IOMNP4 1/5.5 7.2 bubbling air
Table 2.1: Experimental conditions used for to thermal decomposition of FeOOH Figure 2.1: Heating rate ramp for the thermal decomposition reaction of FeOOH.
hematite (PDF 24-0072) (Figure 2.2). The quantification of each phase was obtained analyzing the diffraction pattern by the Rietveld method. The same procedure was followed for all the phase quantification data reported in this chapter.
30 40 50 60 70
(111) (200) (220)
Figure 2.2: XRD patterns of samples a) IOMNP1, b) IOMNP2, c) IOMNP3, d) IOMNP4. The black bars correspond to the reference magnetite pattern (PDF 89-0691), the red bars correspond to the reference hematite pattern (PDF 24-0072), the blue bars correspond to the reference wüstite pattern (PDF 01-1223).
The presence of the hematite phase is undesired since it negatively affects the magnetic properties of the final product; indeed, hematite is characterized by a transition temperature, known as Morin transition, at TM=263-267 K; below TM
hematite is purely antiferromagnetic and above TM is weakly ferromagnetic .
Since for biomedical application we need MNPs with a high magnetic moment, the presence of the hematite phase represents a great drawback.
In order to obtain the magnetite phase only, the reaction was repeated by performing three experiments in a four-fold diluted reaction mixture at a 1:5.5 precursor/surfactant ratio and varying the atmosphere reaction.
Sample IOMNP2 was obtained by accomplishing the reaction under inert N2 atmosphere. In this case no evidence of the hematite secondary phase was
observed in the XRD pattern. However, the pattern reveals the presence of a large amount of another parasitic phase: in fact the Rietveld analysis reveals the nanopowder is composed by a 63% of magnetite and 37% of wüstite, as it clearly appears from the appearance of three peaks, which can be attributed to the (111),
(a) (b) (c) (d)
(200) and (220) families of planes of the cubic face centered structure of wüstite over the characteristic pattern of magnetite. The disappearance of the hematite (Fe2O3) phase replaced by wüstite (FeO) can be imputed to the higher amount of
reducing agents, like CO and H2 produced during the thermal decomposition of the
organic ligand due to the lower precursor/surfactant ratio . Since bulk wüstite is paramagnetic at room temperature and presents an antiferromagnetic ordering below 200 K, similarly to hematite it reduces the magnetic moment of the MNPs.
Figure 2.3 : TEM image of sample IOMNP2. In the inset the size distribution evaluated over 550 MNPs is reported. The two distributions are centered at 17.9 ± 3.8 nm and 21.0 ± 3.3 nm.
Sample IOMNP2 showed the presence of a double population with two distributions centered at 17.9 ± 3.8 nm and 21.0 ± 3.3 nm, respectively, as highlighted in the inset of Figure 2.3. Despite the sample displayed a good homogeneity in terms of shape (almost all the MNPs are spherical), the presence of a double population and the large size are not appropriate to our purposes.
In order to promote the oxidation of Fe(II) to Fe(III) the reaction was first repeated under air atmosphere (sample IOMNP3) and then with air bubbled directly into the reaction mixture ( sample IOMNP4).
The XRD pattern of sample IOMNP3 still shows the presence of the mixed phase magnetite/wüstite but the percentage of magnetite phase increased to 78% (the rest 22% being wüstite). The efficacy of a more oxidant atmosphere was
5 10 15 20 25 30 35 0 10 20 30 40 50 60 70 80 C o u n t Size (nm)
demonstrated by the XRD pattern of sample IOMNP4 that displays the complete disappearance of wüstite phase, albeit it is possible to find a 17% of hematite detectable from the peak assigned to (104) family of planes while the percentage of the magnetite phase was found equal to 83%.
Figure 2.4 : Representative TEM image of sample IOMNP3 (d= 9.5 ± 1.7 nm). In the inset the size distribution evaluated over 500 MNPs is reported.
0 4 8 12 16 20 0 20 40 60 80 100 120 C o u n t Size (nm)
Interestingly, sample IOMNP3 retained an almost spherical shape such as sample IOMNP2, but the mean size decreased to 9.5 ± 1.7 nm despite the reaction atmosphere was the only experimental parameter changed (Figure 2.4). This result confirmed the strong dependence of the product's properties on the adopted experimental conditions.
Figure 2.5 : TEM image of sample IOMNP4(d= 9.4 ± 4.3 nm). In the inset the size distribution evaluated over 300 MNPs is reported.
In Figure 2.5 a representative TEM image of sample IOMNP4 is shown. In this case the shape is very irregular and many large aggregates were formed. The inset in Figure 2.5 is a proof of the great polydispersity achieved in this sample (the mean size measured was found equal to 9.4 ± 4.3 nm). In conclusion, although the "bubbling-air" method has proven useful to avoid the formation of wüstite, it still presents some problems: indeed, the flow of air into the reaction mixture interfered with the correct increasing temperature rate causing a lowering of the temperature up to 250°C, which in turns produced a bad control on MNPs growth. Also the stirring rate is negatively affected, worsening the control on the final size and size distribution of the MNPs. Moreover, neither the use of bubbling air during the reaction led to the formation of a unique crystal phase.
-10 -5 0 5 10 15 20 25 30 0 10 20 C o u n t Size (nm)
22 2.2 Synthesis with iron(III) oleate
Since the results obtained using FeOOH were not satisfactory, an attempt was performed by replacing the substrate for the thermal decomposition reaction with iron(III) oleate (Fe(ole)3). The use of this precursor is a versatile method
which allows tuning the mean size of MNPs by simply varying the experimental parameters like the heating rate ramp, the Fe(ole)3/oleic acid ratio and the reagents
concentration. It is worth to note that Fe(ole)3 is not commercially available and
thus need to be synthesized . In our case we used a well established procedure based on the reaction of FeCl3∙6H2O with sodium oleate (NaOle) according to the
Scheme 2.1 : Scheme for the synthesis of iron (III) oleate.
Fe(ole)3 was used in the thermal decomposition reaction in the presence of
oleic acid as surfactant in a 1:3 precursor/surfactant ratio, using 1-octadecene as solvent.
Figure 2.6: Heating rate ramp for the thermal decomposition reaction of Fe(ole)3.
The reaction was performed under inert atmosphere (N2) and after 4h of
reflux the MNPs were recovered by magnetic decantation and purified by several washing/precipitating steps (sample OlMNP1).
TEM images (a typical example is shown in Figure 2.7) demonstrate that the synthesized MNPs have a spherical shape and a mean diameter of 16.1±1.1 nm with a extremely narrow size distribution.
Figure 2.7 : TEM image of OlMNP1 (d = 16.1± 1.1 nm) . In the inset the size distribution evaluated over 550 MNPs is reported.
5 10 15 20 25 0 100 200 C o u n ts Size (nm)
30 40 50 60 70
Figure 2.8 : XRD pattern of OlMNP1. The the black bars correspond to the reference magnetite pattern (PDF 89-0691), the blue bars correspond to the reference wüstite pattern (PDF 01-1223).
However, the XRD pattern of sample OlMNP1, reported in Figure 2.8 shows, also in this case the presence of two phases, which after the Rietveld analysis can be attributed to magnetite (74%) and wüstite (26%). As previously stated, wüstite affects negatively the magnetic properties of the MNPs since, due to his antiferromagnetic character, it lowers the total magnetic moment of the MNPs. In order to eliminate this parasitic product, an attempt of oxidizing wüstite by a heating treatment of the MNPs in an oven under air atmosphere at different temperatures, (T = 65°C, 90°C, 140°C), and different time (t = 24 h, 48 h at T = 65 °C) was performed. The obtained results are resumed in Table 2.2, where the phase content evaluated from the analysis of the XRD patterns is reported.
30 40 50 60 70
Figure 2.9 : XRD pattern of sample OlMNP1 before and after the heating treatment. a) as prepared MNPs; b) after heating treatment at 65°C for 24h; c) after heating treatment at 65°C for 48h; d) after heating treatment at 90°C for 24h; e) after heating treatment at 140°C for 24h. The black bars correspond to the reference magnetite pattern (PDF 89-0691), the red bars correspond to the reference wüstite pattern (PDF 01-1223)
Comparing the XRD patterns of sample OlMNP1 before and after the heating treatments it is possible to observe a gradual increase of the magnetite phase on increasing temperature up to 90°C (Figure 2.9). Indeed, heating the sample at that temperature, the wustite content decreases to 7%. Then, a further increase in temperature does not produce any significant variation in the relative amounts of the two magnetic phases. On the other hand, also increasing the heating time does not allow to completely eliminate wüstite (Table 2.2).
(a) (b) (c) (d) (e)
Heating treatment Magnetite content Wüstite content
65°C - 24h 85% 15%
65°C - 48 h 90% 10%
90°C - 24h 93% 7%
140°C - 24h 92% 8%
Table 2.2 : Magnetite and wüstite contents in sample OlMNP1 after the heating treatment..
Moreover, the average diameter of the sample oxidized at 90°C, evaluated by using the Scherrer's formula, was 8.3(2.4) nm pointing out that the temperature at which oxidation take place is not large enough to convert the iron oxide into crystalline ferrite . It is worth to note that the peak broadening of the XRD pattern negatively affected the quality of the fit used for determination of crystallites size as well as indicated the low crystallinity of this sample.
The magnetic properties of OlMNP1 treated at 90°C, OlMNP1@90, for 24h were investigated recording the hysteresis loop at 2.5 K and 300 K in the 5 T range (Figure 2.10) An open hysteresis loop was measured at 2.5 K with a coercive field µ0H of 52 mT and a reduced remnant magnetization M0T/M5T, of 0.30. No
magnetic irreversibility was observed at 300 K, indicating that the blocking temperature, i.e. the temperature at which the nanosystem switches from a blocked to a superparamagnetic state is smaller than room temperature. The magnetization was almost saturated at the highest measuring field of 5T reaching a value of 53 Am2Kg-1 at 2.5 K and then it slightly decreases at room temperature down to 50.5 Am2Kg-1.
27 -6000 -4000 -2000 0 2000 4000 6000 -60 -40 -20 0 20 40 60 2.5 K 300 K M ( Am 2 Kg -1 ) 0H (mT) -50 -25 0 25 50 -20 -10 0 10 20
Figure 2.10 : Hysteresis loop recorded at 2.5K (blue dotted line) and at 300 K (red dotted line) and corresponding enlargement of the low field region for sample OlMNP1@90.
The saturation magnetization is lower than the bulk value of 90 Am2Kg-1 . This effect can be attributed both to the presence of the antiferromagnetic wüstite phase and to the occurrence of surface structure defects that can lead to magnetic disorder and hence to a global decrease of the magnetization.
In order to obtain MNPs with a higher magnetic moment the oxidation procedure was then modified replacing the heating treatment in oven with one in solution. To this aim sample OlMNP1 was dissolved in 1-octadecene in the presence of oleic acid so as to obtain a stable suspension. A flux of air was then bubbled into the reaction mixture which was heated up to T = 290°C at a rate of 17°C/min. At the end of the oxidation treatment the MNPs were magnetically decanted and washed several times in order to remove the excess of surfactant.
The XRD pattern of the as obtained MNPs confirmed the efficacy of the oxidation process showing the complete disappearance of the wüstite phase (Figure 2.12).
30 40 50 60 70
Figure 2.12 : Comparison between XRD patterns of (a) mixed phase MNPs synthesized from Fe(ole)3,
(b) OlMNP1@90, oxidized in oven at 90°C for 24h, (c) OlMNP1@290, oxidized in 1-octadecene solution at 290°C with bubbling air.
Moreover, the peak broadening is significantly reduced in this last sample, (the average size of the coherent scattering dominion was estimated to be 12.5(0.3) indicating the crystal quality was significantly improved by the heating treatment carried out in solution.
Substrate Mixed phase MNPs
Surfactant Oleic acid
Figure 2.11 : Experimental conditions adopted for the oxidation of the mixed phase MNPs.
(a) (b) (c)
29 -6000 -4000 -2000 0 2000 4000 6000 -100 -75 -50 -25 0 25 50 75 100 M ( Am 2 Kg -1 ) 0H (mT) MH 300K hyst 2.5K -40 -20 0 20 40 -50 0 50
Figure 2.13 :Hysteresis loop of OlMNP1@290, oxidized in 1-octadecene solution at 290°C with bubbling air, recorded at 2.5K (blue dotted line) and at 300 K (red dotted line) and corresponding enlargement of the low field region.
The hysteresis loop at 2.5 and 300 K of OlMNP1@290 are shown in Figure 2.13. An open hysteresis loop was measured at 2.5 K with a coercive field µ0H of 31 mT
and a reduced remnant magnetization M0T/M5T, of 0.47, while no magnetic
irreversibility was observed at 300 K. Unlike OlMNP1@90, the magnetization is almost saturated at the highest measuring field of 5 T reaching a value of 89 Am2Kg-1 at 2.5 K and 83 Am2Kg-1 at 300 K, very close to value of bulk magnetite, confirming the high crystallinity of the MNPs achieved by this method.
The hyperthermic properties of both oxidized samples, OlMNP1@90 and OlMNP1@290, were investigated recording the temperature kinetic curve of a toluene solution when exposed to an alternating magnetic field with amplitude 17 KAm-1 and frequency 183 KHz. The field parameters were set to stay below the human tolerance threshold, commonly assumed to be given by H0∙ν < 2 - 5∙109
. Larger amplitude or frequency may induce deleterious responses of living tissues and undesired side effects.
The hyperthermic efficiency of a given material is normally evaluate by the so-called Specific Absorption Rate, SAR, which is a measure of the absorbed power for mass unit . The SAR can be evaluated by calorimetric technique, i.e. by measuring the temperature increase ΔT in the interval of time Δt of field
application, using the formula , where, mMe is the total mass of metal, mi is the mass of the i-species present in the sample and Cpi its specific heat. Since the measurements are carried out in non adiabatic conditions, the ΔT / Δt values were extrapolated from the initial slope (t→ 0) of the temperature kinetic curves. Moreover, the time elapse Δt is chosen much shorter than the time constant of the external thermalization circuit.
The SAR values found for OlMNP1@90 and OlMNP1@290 were 4 Wg-1 and 24 Wg-1, respectively (Figure 2.14). The difference in the heat dissipation efficacy among the two samples is a further confirmation that the oxidation process carried out at low temperature led to poor crystallinity, low magnetic moment and hence to bad hyperthermic properties.
100 150 200 250 300 350 400
Figure 2.14 :Temperature kinetics of MNPs colloidal solutions in toluene : OlMNP1@90 (red, 1.2 % w/w) and OlMNP1@290 (black, 0.9 % w/w) during the exposure to the alternating magnetic field (17.0 kA/m, 183 kHz). t T m c m SAR Me i pi i
31 2.3 Synthesis of magnetite MNPs with Iron Acetylacetonate
As we have previously seen, the thermal decomposition of Fe(ole)3
followed by an oxidation step can provide a final product with suitable structural an physical properties. However, despite of this positive aspect, this method still had some drawbacks that may affect its reproducibility. For instance, it has been recently shown that the properties of the final MNPs are dependent upon aging of the precursor . Moreover, the use of a two steps process may be critical for the reproducibility. Therefore, we explored a third approach which uses iron(III) acetylacetonate as a precursor.
Iron(III) acetylacetonate (Fe(acac)3) is a widely used precursor for the
synthesis of magnetite MNPs . However, a major drawback is represented by the difficulties in obtaining MNPs with size larger than 8-9 nm, in a single reaction step. However, it is known from the literature that, in order to have a sizable heating at magnetic field tolerable by human being, iron oxide MNPs must be at least larger than 10 nm . In order to overcome this limitation we first attempted to increase the average size using the so-called seed mediated growth approach. This method consists in preparing small MNPs to be used as seeds to grow larger MNPs in a following thermal decomposition reaction with a further addiction of Fe(acac)3 .
As an alternative approach, we explored the modification of experimental parameters from the solvent to the heating rate ramp, to increase the average size without compromising neither the crystalline quality, nor the magnetic properties.
2.3.1 Synthesis of MNPs exploiting the seed mediated growth process
The synthesis of magnetite MNPs exploiting the seed mediated approach starting from Fe(acac)3 as precursor was performed as follows: first nearly cubic
iron oxide MNPs, IAMNP1, with an average size of 7.6 ± 0.7 (Figure 2.15) nm were synthesized by thermal decomposition of Fe(acac)3 in 1-octadecene and with
Figure 2.15 :TEM image of IAMNP1 (d = 7.6 ± 0.7 nm) used for the seed mediated growth process. In the inset, the size distribution evaluated over 300 MNPs is reported.
Then, the size of the inorganic core was increased by reacting the former MNPs with more Fe(acac)3 under the same experimental conditions. TEM images
of the final product IAMNP2 show that an almost cubic shape was retained while the average size calculated along the diagonal increased to 11.3 ± 1.3 nm (Figure 2.16). 0 2 4 6 8 10 12 14 0 20 40 60 C o u n ts Size (nm)
Figure2.16 : image of IAMNP2 (d = 11.3 ± 1.2 nm) after the seed mediated growth process. In the inset the size distribution evaluated over 600 MNPs is reported.
The position and the relative intensity of all peaks observed in the powder XRD pattern (Figure 2.17) well match those of the fcc spinel structure of standard magnetite (PDF 19-0629), However, the lattice parameter, a, is 8.382(5) Å, much closer to that of magnetite (8.396 Å) than to maghemite (8.346 Å). Notably, no evidence of the presence of wüstite was found in the XRD pattern. The average diameter, evaluated by using the Scherrer’s formula, was 11.5±0.8 in a good agreement with the particle sizes observed in TEM images, pointing out the single crystal nature and the high crystallinity of the MNPs.
2 4 6 8 10 12 14 16 18 20 0 25 50 75 100 C o u n ts Size (nm)
34 25 30 35 40 45 50 55 60 65 70 (440) (511) (422) (400) (311)
Figure 2.17 : Powder X-Ray Diffraction patterns of MNPs (a) IAMNP1, before and (b) IAMNP2, after the seed-mediated growth step. The black bars correspond to the reference magnetite pattern (PDF 19-0629).
The magnetic properties of a colloidal solution of the MNPs in heptane were investigated both as a function of temperature and magnetic field. Since these MNPs were used as multivalent scaffold for the functionalization with the α-Tn antigen mimetic, as it will be described in detail Chapter 3, their magnetic behaviours were deeply investigated. The temperature dependence of the magnetization recorded after zero-field cooling (ZFC) and field-cooling (FC) procedures is reported in Figure 2.18a. It displays the thermal irreversibility characteristic of an ensemble of randomly oriented single domain MNPs :at room temperature all the particles are in the superparamagnetic regime, consistently with the relatively small size of the MNPs, while below ca. 100 K the two magnetization curves split, indicating the beginning of the freezing process of the MNPs magnetic moment. The blocking temperature, which at first approximation can be identified with the temperature of the maximum of the ZFC curve, was 50 K, which well agrees with that expected for magnetite MNPs of 11-12 nm . Accordingly, an open hysteresis loop with a coercive field, HC, of 34
mT, and reduced remnant magnetization, M0T/M5T, equal to 0.49 was measured at
low temperature (2.5 K), while no magnetic irreversibility appears when the loop
was measured above the blocking temperature (at 150 K and at room temperature, Figure 2.18b). 0 50 100 150 200 250 300 0 5 10 15 20 25 30 35 FC ZFC M (A m 2 kg -1 ) Temperature (K) (a) -6000 -4000 -2000 0 2000 4000 6000 -80 -60 -40 -20 0 20 40 60 80 -80 -40 0 40 80 -40 -20 0 20 40 M (Am 2kg -1) 0H (mT) (b)
The magnetization was almost saturated at the highest measuring field of 5 T (the difference between the values measured at 5 T and those extrapolated from the fit of the high field data point to the empirical law M = MS+a/H +b/H2 is ca. 1
%) reaching 75 Am2/kg at 2.5 K and then slightly decreasing on increasing temperature. The saturation magnetization resulted close to the literature value of the corresponding bulk materials confirming the single crystal nature and the high cristallinity of the inorganic cores.
0 50 100 150 200 250 300 0,0 0,5 1,0 1,5 ' (4 *1 0 -3m 3/k g ) T (K) (a) 0,00 0,05 0,10 0,15 0,20 0,25 0,30 0,35 " (4 *1 0 -3 m 3 /k g ) 0,022 0,024 0,026 0,028 0,030 0,032 -9 -8 -7 -6 -5 -4 -3 -2 -1 (b) ln ( ) Tmax-1 (K-1 ) KV/kB = 863 18 K 0 = 310-13 210-13 s
Figure 2.18 : (a) Temperature dependence of the ZFC and FC magnetizations collected on a colloidal solution of the surfactant coated MNPs in heptane with a probe field of 5 mT. (b) Hysteresis loops recorded at 2.5 K (red), 150 K (black) and 300 K (blue curve) and corresponding enlargement of the low field region (inset).
Figure 2.19 : AC susceptibilities and Arrhenius plot. (a) Temperature dependence of in-phase, χ’, (full symbols) and out-of-phase, χ", (open symbols) AC susceptibilities. Data were collected at 6 log-spaced frequencies in the 1-1000 Hz range. (b) Arrhenius plot of the experimental relaxation time and best fit line.
The relaxation dynamics of the magnetic moment was further investigated by temperature-dependent AC susceptibility measurements at variable frequency (1-1000 Hz, Figure 2.19). Both the in- and out-of-phase components of the magnetic susceptibility exhibited frequency-dependent maxima characteristic of a blocking process. The blocking temperatures obtained from the maxima of the out-of-phase component of the magnetic susceptibility, χ”, for diﬀerent observation times τ = 1/2πν, where ν is the frequency of the ac ﬁeld, can be effectively ﬁtted to an Arrhenius law, = τ0 exp(KV/kBT), where K is the magnetic anisotropy energy density, V is the particle volume, τ0 the attempt time and kB the Boltzmann constant. The best-ﬁt parameters found were 3∙10-13 ± 2∙10-13s for the pre-exponential factor, τ0, and 863 ± 18 K for the reversal energy barrier, KV/kB, which, considering the average volume obtained from the analysis of TEM images, corresponds to K ≈ 2.2·104 J/m3. Interestingly, no anomalies in the χ' vs. T curves were observed nor at the melting point of heptane (183 K), or at higher temperature, a result which indicates that at room temperature, at least in the investigated time window, the reversal of the magnetization is mainly driven by the Néel mechanism, rather than by the mechanical rotation of the whole MNPs. This result is particularly important in view of the possible application of these nanosystems in clinics. Indeed, since in our case the relaxation is determined by intrinsic magnetic parameters rather than on extrinsic parameters, as it would have been if the relaxation were dominated by Brownian motion of the nanoparticle, we can reasonably assume the observed behaviour will not change once the particles will be introduced in human tissue.
In order to evaluate the heat dissipation efficiency we recorded the temperature kinetic curve of the heptane colloidal solution when exposed to an alternating magnetic field with amplitude H0 = 11.0 kA/m and frequency ν = 183
kHz. Also in this case, the field parameters were set to stay below the human tolerance threshold, commonly assumed to be given by H0∙ν < 2 - 5∙109 A∙m-1∙s-1
. The application of this alternating field on a 1.9 % w/w solution of the MNPs for 5 minutes produced a sizable temperature increase of ca. 9°C corresponding to a SAR value of ca. 10 W/g, as shown in Figure 2.20. Although this value is low if compared to data reported in the literature (which are however, commonly obtained using much higher, clinically unexploitable field amplitudes) it corresponds to a sizable heating efficiency, which suggests this material can be possibly used as heat mediator in adjuvant antitumoral therapy.
37 0 100 200 300 400 500 18 20 22 24 26 28 30 H0=0 H0=11 KA/m T ( °C ) t (s) H0=0
Figure 2.20 : Temperature kinetics of a colloidal solution of iron oxide MNPs during the exposure to the alternating magnetic field (11.0 kA/m, 183 kHz).
The low SAR value can be attributed both to the small size of the MNPs (which, for magnetite is close to the lower limit for producing sizable heat dissipation at these field parameters) and the presence of strained lattice regions that can alter the magnetic structure of the crystals creating a discrepancy between the crystal size and the effective magnetic volume. Pellegrino et al. had demonstrated that the origin of this crystal strain is strictly correlated with the seed mediated growth method . This particular drawback turned our efforts toward the development of a procedure to synthesize larger magnetite MNPs in a single reaction avoiding any seeded process.
2.3.2 Synthesis of larger magnetite MNPs from iron(III) acetylacetonate
As mentioned in the previous paragraph, the synthesis of magnetite MNPs with size above 10 nm without exploiting the seed mediated growth process is often challenging and hard to achieve. Nevertheless, due to the intrinsic limitation of the seed growth method, we decide to make an effort to verify if by changing various experimental parameters in the thermal decomposition of Fe(acac)3,
ranging from the composition of the reaction mixture to the heating rate ramp, were possible to get magnetite MNPs with average size above 10 nm.
To realize this goal we maintained oleic acid and oleylamine as surfactants but changed the precursor/surfactant ratio and the reagents concentration. Both parameters are important in the nucleation and growing phase . Differently from the previously described synthesis, in this case the employment of 1,2-hexadecanediol was avoided because, as demonstrated by Barron et al., it promotes the formation of small sized MNPs, meanwhile not providing any advantage in terms of polydispersity index . Moreover, the reaction solvent was changed from 1-octadecene (b.p. 320°C) to benzyl ether (b.p. 298°C) thus facilitating the MNPs purification from the reaction mixture. The removal of octadecene residues is indeed more difficult causing a larger consumption of hexane and ethanol for the purification process.
The first two experiments were performed with a Fe(acac)3/oleic
acid/oleylamine ratio equal to 1 : 4.5 : 3.5 in 50 mL of benzylether, varying ti (the
time spent to reach reflux condition) and tr (reflux time) in the heating rate ramp as
described in Figure 2.21.
Figure 2.21: Heating ramp employed for the synthesis of samples IAMNP3 and IAMNP4 where ti
represents the time spent to reach reflux condition and tr the reflux time.
The XRD patterns of both samples, shown in Figure 2.22, well match that of the fcc spinel structure of magnetite (PDF 88-0315) and no traces of any other crystal phase appears confirming that the use of Fe(acac)3 as precursor avoid the
formation of any undesired phase like wüstite or hematite.
IAMNP3 : ti=50' and tr=50'
30 40 50 60 70
Figure 2.22 : XRD patterns of samples IAMNP3 and IAMNP4. In red the reference pattern of magnetite (PDF 88-0315) is shown.
From the TEM images shown in Figure 2.23 it is possible to observe that sample IAMNP3 was mostly composed by faceted polyhedral nanocrystals with an average size of 20.7 ± 2.6 nm whereas MNPs in sample IAMNP4 had an almost spherical shape with a mean size of 7.3 ± 2.0 nm: the transition from the spherical to a faceted polyhedral morphology is usually found in MNPs bigger than 15-16 nm. In the case of sample IAMNP3 the longest ti and tr times favored the growth
step with respect to nucleation, thus leading to the formation of MNPs bigger than 20 nm, grown along the most favorable crystallographic directions. Conversely, the shortening of ti in sample IAMNP4, smaller MNPs were achieved. In both cases
the large size distribution can be attributed to the inadequate separation between the nucleation and the growing phases.